advertisement

arXiv:cond-mat/0309716v1 [cond-mat.supr-con] 30 Sep 2003 Vortex Lattice in Bi2Sr2CaCu2O8+δ Well Above the First-Order Phase-Transition Boundary J. H. S. Torres ∗, R. Ricardo da Silva 1, S. Moehlecke, Y. Kopelevich Instituto de Fı́sica “Gleb Wataghin”, Universidade Estadual de Campinas, Unicamp 13083-970, Campinas, São Paulo, Brasil Abstract Measurements of non-local in-plane resistance originating from transverse vortexvortex correlations have been performed on a Bi2 Sr2 CaCu2 O8+δ high-Tc superconductor in a magnetic field up to 9 T applied along the crystal c-axis. Our results demonstrate that a rigid vortex lattice does exist over a broad portion of the magnetic field – temperature (H-T) phase diagram, well above the first-order transition boundary HF OT (T). The results also provide evidence for the vortex lattice melting and vortex liquid decoupling phase transitions, occurring above the HF OT (T). Key words: A. Superconductors, D. Flux pinning and creep, D. Phase transitions PACS: 74.72.Hs, 74.60.Ge The knowledge of the magnetic field – temperature (H-T) phase diagram is a cornerstone of the phenomenological description of superconductors. The H-T phase diagram of conventional type-II superconductors is well known. In the Meissner-Ochsenfeld state, the surface currents screen the applied magnetic field. Above the lower critical field Hc1 (T) the applied field penetrates the superconductor in the form of an Abrikosov vortex lattice which persists up to the upper critical field Hc2 (T), where the superconductivity vanishes in the bulk of the sample. On the other hand, in high-temperature superconductors (HTS), due to strong thermal fluctuations, the occurrence of the vortex lattice melting phase transition at Hm (T) ≪ Hc2 (T) has been predicted (for review articles see Ref. [1] and Ref. [2] and references therein). Since then, considerable efforts have been dedicated to identifying the melting transition in experiments. At present, it is widely believed that the vortex ∗ Corresponding author. Email address: [email protected] (J. H. S. Torres). 1 Also at FAENQUIL, 12600-000, Lorena, SP, Brasil Preprint submitted to Elsevier Science 2 February 2008 lattice melting is related to a first-order transition (FOT) occurring, e. g. in Bi2 Sr2 CaCu2 O8 (Bi2212) high-Tc superconductor, at a very low field HF OT (T) [3]. Thus, at T ∼ Tc /2 the HF OT ∼ 500 Oe, which is several orders of magnitude smaller than Hc2 ∼ 100 T. At the FOT, the equilibrium magnetization jump ∆Meq (H,T) takes place [3], which, together with the Clausius-Clapeyron equation, would imply the occurrence of the entropy jump ∆s(H,T) associated with the transition. However, an alternative explanation for the magnetization (entropy) jump due to first-order depinning transition is also possible [4]. At this floating-type transition, the vortex lattice does not melt but does the opposite, it decouples from the atomic lattice becoming more ordered. The entropy jump associated with the vortex lattice floating transition has recently been obtained in Monte Carlo simulations by Gotcheva and Teitel [5]. The occurrence of the floating vortex solid phase situated between a pinned vortex solid and a vortex liquid state has been proposed two decades ago by Nelson and Halperin [6]. The FOT in HTS is accompanied by a sudden increase in the electrical resistivity [7] which demonstrates the sharpness of the vortex depinning onset. A sharp resistive magnetic-field-induced depinning transition separating disordered (low-field) from ordered (high-field) vortex states has recently been reported for NbSe2 , suggesting the first-order nature of the depinning transition [8]. In Bi2212, the in-plane non-local resistance, the indication of a finite shear stiffness of the vortex matter, has been measured above the FOT by Eltsev et al.[9]. It has been concluded, however, that the strong transverse vortex-vortex correlations take place in the vortex liquid phase [9]. In the present work, we report the observation of in-plane non-local resistance in Bi2212 in an applied magnetic field up to H = 9 T. The obtained results demonstrate that the vortex lattice does exist over a broad portion of the H-T phase diagram above the FOT boundary. The resistance measurements were performed on a l × w × t = 1.94 × 0.28 × 0.03mm3 size Bi2212 single crystal grown using the self-flux method. The crystal characterization details as well as dc magnetization measurements have been presented elsewhere [10]. The crystal zero-field superconducting transition temperature T0c = 87.7 K has been determined from the maximum of the temperature derivative dR/dT. The resistance measurements were made using PPMS (9T magnet) Quantum Design commercial equipment in magnetic fields applied along the crystal c-axis. The FOT boundary has been obtained by means of dc magnetization M(H,T) measurements (H k c - axis) with the SQUID magnetometer MPMS5 (Quantum Design). We used the line-electrode geometry [11,12,13] to study the non-local in-plane resistance. Six silver epoxy electrodes with contact resistance ∼ 1Ω were patterned on one of the main surfaces of the crystal, as shown in the inset of Fig.1, with a separation distance s ∼ 180 µm. In the experiments, the dc current I14 was applied between the current leads 1 and 4, and the voltage was measured 2 1.0 0.8 R14,23 Rik,lm (Ω) 0.6 0.4 0.2 R14,56 0.0 -0.2 0 50 100 150 200 250 300 T (K) Fig. 1. Temperature dependences of “primary” R14,23 = V14,23 /I14 and “secondary” R14,56 = V14,56 /I14 resistances measured in applied magnetic field H = 9 T and I14 = 1 mA; dotted line is the “parasitic” contribution to R14,56 , resulting from the current distribution effect as estimated from Eq. (1). Inset shows the geometry of the experiment. simultaneously in both the applied current part of the crystal V23 and outside this region V56 . Figure 1 shows temperature dependences of both “primary” R14,23 = V14,23 /I14 and “secondary” R14,56 = V14,56 /I14 resistances obtained in applied field H = 9 T and for I14 = 1 mA. As can be seen from Fig. 1, R14,56 is negative in the normal state, and shows a crossover to positive values below a certain temperature within the superconducting state. The negative R14,56 , which develops with the increase of temperature is related to the current distribution through the crystal thickness, i. e. has a local origin. Using the equation derived by van der Pauw [14] R14,56 = −(wR14,23 /πs) ln[(a + b)(b + c)/b(a + b + c)], (1) where a, b, and c are distances between electrodes 1 and 4, 4 and 5, 5 and 6, respectively, we obtain the R14,56 (T), depicted in Fig. 1 by a dotted line. The agreement between calculated and measured R14,56 (T) is rather good, taking into consideration the strong crystallographic anisotropy of Bi2212, the finite width of the electrodes, and a probable distortion of the electrical potential along the line contacts. Shown in Fig. 2(a) and Fig. 2(b) are R14,23 (T,H) and 3 (a) R14,23 (Ω) 0.6 0.3 0.0 H H H H H H H H H (b) R14,56 (Ω) 0.05 = = = = = = = = = 0 1 2 3 4 5 6 7 9 T T T T T T T T T 0.00 20 40 60 80 100 120 T (K) Fig. 2. “Primary” resistance R14,23 (T) (a) and “secondary” resistance R14,56 (T) (b) measured at various applied magnetic fields and I14 = 1 mA. Arrows (b) indicate the field-dependent temperature Tmax (H), where a single peak in R14,56 (T,H) takes place. Symbols in (a) and (b) correspond to the same fields (b). R14,56 (T,H), respectively measured at various applied magnetic fields. As can be seen from Fig. 2(b), the positive “secondary” resistance R14,56 (T,H) emerges and increases with field. For H > 2 T, the R14,56 (T,H) shows a well defined peak at the temperature Tmax (H), which decreases with the field increase. The results presented in Figs. 3–5 unambiguously demonstrate that the positive contribution to R14,56 (T,H) originates from the non-local resistance, i. e. is not related to the current distribution effects. Figure 3 (a, b) shows R14,56 (T) measured with I14 = 100 µA and I14 = 1 mA for H = 2 T [Fig. 3(a)] and H = 4 T [Fig. 3(b)]. In Fig. 4 we plotted ∆R14,56 = R14,56 (I14 = 100 µA) – R14,56 (I14 = 1 mA) and ∆R14,23 = R14,23 (I14 = 100 µA) – R14,23 (I14 = 1 mA) versus temperature. From Fig. 3 and Fig. 4 we note that (1) as the temperature approaches Tmax (H) from below, R14,56 4 40 50 60 70 20 (a) 10 R14,56 (mΩ) H=2T 0 (b) 30 H=4T 20 45 50 55 60 65 T (K) Fig. 3. “Secondary” resistance R14,56 (T) measured with I14 = 100 µA (solid symbols) and I14 = 1 mA (open symbols) for H = 2 T (a) and H = 4 T (b). becomes larger for smaller applied current, and the R14,56 (T,H) peaks at T ≈ Tmax (note that ∆R14,23 ≈ 0, i. e. R14,23 is current-independent at the studied temperatures), (2) the current dependence of R14,56 persists up to ∼ Tc , i. e. is essentially related to the superconducting state. Note also that the current effect vanishes with field, so that it is negligible for H ≥ 6 T. At T < Tmax (H) the ratio R14,56 /R14,23 increases with temperature, as shown in Fig. 5, for several studied fields. All these experimental facts can hardly be understood within a local approach, indeed. Certainly, the large enhancement of the non-local resistance with temperature over a broad temperature interval cannot be accounted for by vortex-vortex correlations in the vortex liquid. On the other hand, the long-range positive non-local resistance can arise from a correlated transverse motion of the vortex lattice [12]. The in-plane vortex-vortex correlations occurring on a millimeter scale have also been detected in Corbino-disk experiments [15,9]. 5 ∆R14,56 3.0 H=2T ∆Rik,lm (mΩ) TC 1.5 0.0 ∆R14,23 -1.5 40 60 80 100 120 140 T (K) Fig. 4. The difference ∆R14,56 = R14,56 (I14 = 100 µA) – R14,56 (I14 = 1 mA) (solid symbols) and ∆R14,23 = R14,23 (I14 = 100 µA) – R14,23 (I14 = 1 mA) (dotted line) versus temperature measured for H = 2 T. 0.4 H=9T H=7T R14,56/R14,23 H=6T H=5T 0.3 H=4T 0.2 25 30 35 40 45 50 T (K) Fig. 5. The “secondary” to “primary” resistance ratio R14,56 /R14,23 vs. temperature obtained with I14 = 1 mA illustrated for several measuring fields. 6 The ratio R14,56 (T)/R14,23 (T) < 1, see Fig. 5, can result from the vortex pinning effect which destroys the long-range positional order in the vortex lattice and, therefore, leads to a depression of the non-local resistance at large distances. As the temperature increases, both R14,56 (T) and R14,56 (T)/R14,23 (T) increase due to a vortex pinning efficiency decrease. Approaching Tmax (H), the ratio R14,56 (T)/R14,23 (T) starts to decrease. On the other hand, the occurrence of the maximum in ∆R14,56 (T) at T ≈ Tmax (H), see Fig. 4, rules out any trivial (i.e. within a local approach) explanation of the R14,56 (T) reduction above Tmax (H). A non-trivial origin of the maximum in R14,56 (T,H) is supported by the observation of a splitting of this maximum into two peaks which takes place below ∼ 1 T, see Fig. 6. The occurrence of two peaks (or hollow) in R14,56 (T,H) at low fields can be understood assuming the “reentrant” enhancement of the vortex pinning efficiency in the temperature interval Tp1 (H) < T < Tp2 (H), which resembles a phenomenon known as “peak effect” (PE) [16,17]. In agreement with the PE occurrence, the increase of the “primary” R14,23 (T,H) resistance slows down at T ≥ T1 ∼ Tp1 , as Fig. 7, where dR14,23 (T,H)/dT vs. T is plotted, illustrates for H = 0.3 T. A similar phenomenon takes place at the temperature T1 (H) just below Tmax (H) in the high-field limit, see Fig. 7 (the second peak in the derivative dR14,23 (T,H)/dT occurring at temperature T2 (H) is related to the superconductor-normal metal transition). In the low-field limit, we have also observed a current-induced suppression of R14,56 (T,H) at T > Tmin (H), see inset in Fig. 6. This implies a similar vortex state occurring above Tmax (H) (high fields) and above Tmin (H) (low fields). The above results are summarized in the magnetic field – temperature (H-T) diagram (Fig. 8) which we discuss now. The FOT boundary obtained by means of dc magnetization measurements (not presented here) is plotted in Fig. 8 together with data from Ref. [7], measured for a similar Bi2212 crystal. It is evident from Fig. 8 that at T ∼ Tc /2, the HF OT (T) is about 100 times smaller than the Hmax (T), implying that the long-range transverse vortex-vortex correlations persist well above the FOT boundary. This fact has a natural explanation, assuming that the floating (depinning) transition is associated with the FOT [4,5,6]. At H < HF OT (T) ∼ Φ0 /λ2ab , the vortex lattice shear modulus decreases exponentially with field c66 ≈ (ε0 /λ2ab )(Hλ2ab /Φ0 )1/4 exp[−(Φ0 /Hλ2ab )1/2 ], whereas at H > HF OT (T), c66 ≈ (ε0 /4Φ0 )H, i. e. c66 linearly increases with field [1,2], where ε0 = (Φ0 /4πλab )2 . This implies that, at H < HF OT (T), the interaction between vortices and the quenched disorder overwhelms the vortex-vortex interaction, leading to a stronger vortex pinning in the low-field regime (note that at H << HF OT (T) the pinned vortex liquid is expected [18]). With the field increase the c66 (H,T) and hence the inter-vortex interaction increase, and the vortex lattice de-couples from the atomic lattice at HF OT (T). Usually, the 7 4 H H H H 3 R14,56 (mΩ) 2 = = = = 0.1 0.2 0.3 0.5 Tp2(H) T T T T Tp1(H) Tmin(H) 1 0 0 -1 -1 H = 0.1 T -2 -2 -3 40 60 65 70 50 75 80 85 60 70 80 T (K) Fig. 6. The “secondary” resistance R14,56 (T) measured for several low (see text) fields with I14 = 1 mA. The inset shows R14,56 (T) measured at H = 0.1 T with I14 = 100 µA (solid symbols) and I14 = 1 mA (open symbols). T1(H) ~ Tmax(H) dR14,23/dT (Ω/K) T1(H) ~ Tp1(H) H=7T 10 -2 T2(H) H=2T 10 H = 0.3 T -3 30 60 90 T (K) Fig. 7. The derivative dR14,23 /dT vs. T demonstrating the slowing-down of the “primary” resistance increase at T ≥ T1 (H) which is situated just below the Tmax (H) at high fields (H ≥ 2 T) and coincides with the Tp2 (H) at low fields (H ≤ 0.5 T). At the temperature T2 (H), transition to the normal state takes place. 8 10 1 H(Tmax) H(T1) H (T) 10 10 0 CROSSOVER REGION H(Tp2) H(Tp1) -1 H(Tmin) 10 HFOT(T) -2 H(T2) 45 50 55 60 65 70 75 80 85 90 T (K) Fig. 8. Magnetic field – temperature (H-T) diagram constructed on the base of experimental results (see text). The first order transition boundary HF OT (T) measured in both this work (2) and Ref. [7] (x) is also shown. depinning transition in HTS is rather sharp [7]. We stress that besides theoretical expectations of a sharp depinning transition [19,20], an experimental evidence of a jumpy-like magnetic-field-induced floating transition has recently been reported [8]. At H > HF OT (T) and low enough temperatures, c66 (H,T) is weakly temperature-dependent. In this regime, the vortex lattice becomes more ordered when the temperature is increased due to the suppression of the vortex pinning efficiency by thermal fluctuations, resulting in the increase of the non-local in-plane resistance with temperature. This observation is in excellent agreement with the second-order diffraction in small-angle neutron scattering experiments [21] which revealed the formation of a more ordered vortex lattice with the temperature increase for intermediate temperatures and magnetic fields. The c66 (H,T) rapidly decreases, however, approaching either the upper critical field Hc2 (T) or the melting phase transition boundary Hm (T) < Hc2 (T). In both cases, the vortex lattice can better adjust the pinning potential [16,17] leading to the reduction of the non-local signal. There are two plausible scenarios which allow us to account for the occurrence of the minimum in R14,56 (T,H) in the low-field regime, see Fig. 6. The first possibility is that thermal fluctuations smear out the pinning potential, improving the vortex lattice which leads to the reentrant increase of R14,56 (T,H) with the temperature increase at T > Tmin (H) [22]. At T = Tp2 (H), the vortex lattice melts or the superconducting order parameter diminishes because of strong fluctuations in its amplitude; both effects will suppress the non-local resistance. On the other hand, the minimum in R14,56 (T,H) occurring at the 9 Tmin (H) can coincide with the melting transition temperature Tm (H) in the presence of quenched disorder [23,24,25]. Then, in a narrow temperature interval above the Tm (H), a shear viscosity due to a finite crossing energy U× (H,T) of the entangled vortex liquid [26,27] can lead to the restoration of the nonlocal resistance. As temperature increases further, the U× (H,T) vanishes [27], and the non-local resistance will be suppressed together with the entangled vortex state at the “decoupling” transition temperature TD (H) = Tp2 (H) > Tm (H), above which vortex fluctuations have a two-dimensional (2D) character. This second scenario agrees with the observed suppression of R14,56 (H,T) at T > Tmin (H) by the applied current, assuming the occurrence of currentinduced vortex cutting [28]. There is also a striking correspondence between the experimental results, see Fig. 9, and the low-field portion of the H-T phase diagram proposed by Glazman and Koshelev [29] for layered superconductors. Indeed, the H(Tmin ) can be described perfectly by a theoretical 3D “melting line” [1,2,29] Hm (T ) ∼ = Φ0 ε20 c4L /(kB T )2 γ 2 , (2) where γ=λc /λab is the anisotropy factor, λc is the out-of-plane penetration depth, and cL = 0.1 – 0.4 is the Lindemann number. The Eq. (2) can be re-written in the form Hm (T ) = B(1 − t2 )2 /t2 , (3) where t ≡ Tm /Tc0 , Tc0 is the mean-field transition temperature, and B = Φ50 c4L /256π 4 (kB Tc0 )2 γ 2 λ4ab (0). The fitting gives B = 1.5 T (see Fig. 9). Taking a dimensional crossover field [29] for our crystal H3D−2D ∼ = Φ0 /(γd)2 ∼ 0.5 T which separates 3D (H < H3D−2D ) and quasi-2D (H > H3D−2D ) vortex fluctuation regimes, we obtain γ ≈ 40 (here d = 15 Å is the distance between weakly coupled CuO2 bi-layers). Then, with λab (0) ∼ 1000 Å, one gets a reasonable value for the Lindemann number cL = 0.23. On the other hand, H(Tp2 ) can be best approximated by the linear dependence (see Fig. 9) HD (T ) = C(Tc − T )/T, (4) which describes the thermally induced 3D-2D vortex liquid decoupling transition in a vicinity of Tc [29]. Here C = αD Φ30 /dkB Tc (4πλc )2 , and αD is some constant. With the fitting parameter C = 4.4 T, one has αD ∼ 1. The apparent crossing of Hm (T) and HD (T) lines seen in Fig. 9 originates from the entering into the critical superconducting fluctuations region (see, e. g., Ref. [30]). For H > 0.5 T, H(Tp1 ) and H(Tp2 ) start to merge and, for H > 2 T, a single 10 0.5 2D VORTEX LIQUID H (T) 0.4 FLUX LINE LIQUID 0.3 0.2 0.1 0.0 65 FLUX LINE LATTICE 70 75 80 85 T (K) Fig. 9. Low-field (H < H3D−2D ) portion of the H-T phase diagram. The solid line corresponds to the equation Hm (T ) = B(1−t2 )2 /t2 , which describes the flux-line-lattice melting phase transition (Eq. (3)); B = 1.5 T, t = Tm /Tc0 , Tc0 = 89 K. The dotted line corresponds to the equation HD (T ) = C(Tc − T )/T (Eq. (4)), which describes the 3D-2D “decoupling” transition in the vortex liquid state; C = 4.4 T, and Tc = 84.1 K. transition in the vortex matter takes place at Tmax (H). For H >> H3D−2D , the theory [29] predicts that Hm (T) approaches the melting temperature of √ −1 2D ∼ an isolated superconducting CuO2 bi-layer Tm = (kB 8π 3) dε0 according to the equation: Hm (T ) ∼ = H3D−2D exp{b[Tm2D /(T − Tm2D )]ν }, (5) where b ∼ 1, and ν = 0.37. Figure 10 demonstrates a good agreement between Eq. (5) and the experimental H(Tmax ) boundary at H > 4 T. The fitting gives H3D−2D = 0.74 T and T2D m = 46.3 K (λab (0) ≈ 1200 Å). Thus, taking the overall data together, we are led to conclude on a possible occurrence of vortex lattice melting and “decoupling” phase transitions associated with H(Tmin ) and H(Tp2 ) low-field boundaries, respectively, as well as on the melting of a quasi-2D vortex solid which takes place along the H(Tmax ) boundary at H ≫ H3D−2D . The current effect on the non-local resistance measured at both T ≥ Tmin (H) and T ≥ Tmax (H), and its vanishing with the field increase, suggests the ocurrence of the entangled vortex liquid for low and intermediate fields. We stress that the results obtained here suggest an enhancement of the vortex pinning in the vortex liquid state, being in 11 8 VORTEX LIQUID H (T) 6 4 VORTEX SOLID 2 0 45 Tm 2D 50 55 60 65 T (K) Fig. 10. The high-field (H > H3D−2D ) portion of the H-T phase diagram; () H(Tmax ), solid line is obtained from Eq. (5) with H3D−2D = 0.74 T, and T2D m = 46.3 K. agreement with Refs. [23,24,25,29]. To summarize, results of the present work provide an experimental evidence for the vortex lattice existence in Bi2 Sr2 CaCu2 O8 well above the first-order transition boundary HF OT (T). For the first time, the H-T phase diagram of the high-Tc superconductor is constructed on the basis of direct probe of transverse vortex-vortex correlations. We gratefully acknowledge valuable discussions with G. Carneiro, P. Esquinazi, E. Granato, V. M. Vinokur, and E. Zeldov. This work was supported by FAPESP, CNPq and CAPES Brazilian agencies. References [1] G. Blatter, M. V. Feigel’man, V. B. Geshkenbein, A. I. Larkin, and V. M. Vinokur, Rev. Mod. Phys. 66, 1125 (1994). [2] E. H. Brandt, Rep. Prog. Phys. 58, 1465 (1995). [3] E. Zeldov, D. Majer, M. Konczykowski, V. B. Geshkenbein, V. M. Vinokur, and H. Shtrikman, Nature 375, 373 (1995). 12 [4] Y. Kopelevich and P. Esquinazi, Solid State Commun. 114, 241 (2000). [5] V. Gotcheva and S. Teitel, Phys. Rev. Lett. 86, 2126 (2001). [6] D. R. Nelson and B. I. Halperin, Phys. Rev. B 19, 2457 (1979). [7] D. T. Fuchs, E. Zeldov, D. Majer, R. A. Doyle, T. Tamegai, S. Ooi, and M. Konczykowski, Phys. Rev. B 54, 796 (1996). [8] Y. Paltiel, E. Zeldov, Y. Myasoedov, M. L. Rappaport, G. Jung, S. Bhattacharya, M. J. Higgins, Z. L. Xiao, E. Y. Andrei, P. L. Gammel, and D. J. Bishop, Phys. Rev. Lett. 85, 3712 (2000). [9] Yu. Eltsev, K. Nakao, S. Shibata, and N. Koshizuka, Proc. Int. Conf. On Materials and Mechanisms of Superconductivity, High Temperature Superconductors VI, Houston, Texas, 2000: Physica C 341-348, 1107 (2000). [10] Y. Kopelevich, S. Moehlecke, J. H. S. Torres, R. Ricardo da Silva, and P. Esquinazi, J. Low Temp. Phys. 116, 261 (1999). [11] H. J. Mamin, J. Clarke, and D. J. Van Harlingen, Phys. Rev. B 29, 3881 (1984). [12] R. Wortis and D. A. Huse, Phys. Rev. B 54, 12413 (1996). [13] Y. Kopelevich, F. Ciovacco, P. Esquinazi, and M. Lorenz, Phys. Rev. Lett. 80, 4048 (1998). [14] L. J. van der Pauw, Philips Research Reports 13, 1 (1958). [15] D. López, W. K. Kwok, H. Safar, R. J. Olsson, A. M. Petrean, L. Paulius, and G. W. Crabtree, Phys. Rev. Lett. 82, 1277 (1999). [16] A. B. Pippard, Philos. Mag. 19, 217 (1969). [17] A. I. Larkin, M. C. Marchetti, and V. M. Vinokur, Phys. Rev. Lett. 75, 2992 (1995). [18] D. R. Nelson, Phys. Rev. Lett. 60, 1973 (1988). [19] A. E. Koshelev and P. H. Kes, Phys. Rev. B 48, 6539 (1993). [20] O. S. Wagner, G. Burkard, V. B. Geshkenbein, and G. Blatter, Phys. Rev. Lett. 81, 906 (1998). [21] E. M. Forgan, M. T. Wylie, S. Lloyd, S. L. Lee, and R. Cubitt, Proc. LT-21: Czechoslovak Journal of Physics 46, 1571 (1996). [22] Vanishing of the critical current above the PE region but slightly below the Hc2(T) was observed in Nb-O classical superconductor ; Y. Kopelevich and S. Moehlecke, Phys. Rev. B 58, 2834 (1998). [23] S. Bhattacharya and M. J. Higgins, Phys. Rev. Lett. 70, 2617 (1993); Phys. Rev. B 52, 64 (1995). [24] C. Tang, X. Ling, S. Bhattacharya and P. M. Chaikin, Europhys. Lett. 35, 597 (1996). 13 [25] E. Granato, T. Ala-Nissila, and S. C. Ying, Phys. Rev. B 62, 11834 (2000). [26] D. R. Nelson and H. S. Seung, Phys. Rev. B 39, 9153 (1989). [27] C. Carraro and D. S. Fisher, Phys. Rev. B 51, 534 (1995). [28] H. Safar, P. L. Gammel, D. A. Huse, S. N. Majumdar, L. F. Schneemeyer, D. J. Bishop, D. López, G. Nieva, and F. de la Cruz, Phys. Rev. Lett. 72, 1272 (1994). [29] L. I. Glazman and A. E. Koshelev, Phys. Rev. B 43, 2835 (1991). [30] A. K. Nguyen and A. Sudbo, Phys. Rev. B 58, 2802 (1998). 14